Tribology in Industrywww.tribology.rs
Abrasive Wear Performances of
Different Polyamides by Response Surface
, A. Denizb
, F. Şahinc
aDepartment of Mechanical Engineering, Faculty of Engineering of Near East University, Near East Boulvard, 99138
Nicosia, TRNC Mersin 10 – Turkey,
bDepartment of Manufacturing Engineering, Faculty of Technology, Gazi University, Besevler-06500, Ankara, Turkey,
cDepartment of Manufacturing Engineering,Faculty of Technology, Gazi University, Besevler-06500, Ankara, Turkey.
Polyamides Abrasive wear Load
Tensile strength RSM method
A B S T R A C T
This study presents the investigation of abrasive wear performances for polyamides using a Response Surface Methodology (RSM). Tests were carried out in a pin-on-disc using various conditions against SiC abrasive cloth. Box-Behnken Design of RSM was adopted to study the effect of control factors like load, speed and tensile strength of the tested samples on the volumetric wear rate. The experimental results indicated that the volumetric wear rate increased with increasing load, speed and decreased with increasing the tensile strength, but material property was more effective than other factors. Furthermore, the results of analysis of variance showed that tensile strength was predominant factor on the abrasive wear rate, followed by load and spindle speed. The contributions of tensile strength, load and speed were about 33.55 %, 24.45 % and 21.87 %, respectively, while the contribution of square and 2-way of interaction was about 3.04 % and 11.23 %, respectively.
© 2019 Published by Faculty of Engineering
Department of Mechanical Engineering, Faculty of Engineering of Near East University, Near East Boulvard, 99138 Nicosia, TRNC Mersin 10 – Turkey.
Due to their combination of higher mechanical, physical, chemical/corrosion resistance and tribological properties in addition to their easy processing, polymers are widely used for numbers of engineering applications such as bearings, bushes, gears, cams, rollers and bearing cages against metals, polymers and ceramics .
Polyamides (PAs) are polymers which contain repeating amide bonds, known as cast nylons. Polyamide PA6 and PA66 are the most widely preferred for engineering and industrial applications such as chemical, mining, ship, package, automotive, manufacturing/mechanical and tribological fields .
When there is contact between the sliding pairs of materials, the friction and wear problems
always takes place. For industry, however, the most of the wear problems encountered are abrasive wear about 60 % of total cost . Abrasive wear, which is the most important one, occurs with the sliding of a hard material over a softer material under load, while surface asperities of harder material remove the softer material .
The wear of polymer is a complex phenomenon that depends upon many factors like types of material, geometries, surface property, mechanical property, crystallinity, glass transition temperature, orientation and test conditions [5-21]. Under dry conditions, significant improvements are achieved for the dry wear of polymer based materials. However, there are a limited numbers of studies related to the abrasive properties of the polymers. Pejakovic et al.  studied the abrasion wear resistance of commercially available selected polymer materials using SiO2 abrasives. The polyethylene-based samples showed the lower wear resistance while the polyurethane-based samples indicated that abrasion behavior depended on both hardness and elongation. Shipway and Ngao  investigated the abrasive wear behavior of polymeric materials and the results indicated that the polymer type determined the wear property. Funda et al.  developed the empirical model using RSM for the prediction weight loss of polyoxymethylen (POM) under abrasive sliding. The weight loss increased with increasing load and sliding distance. Sagbas et al. also investigated the wear behavior of POM in terms of load and sliding distance, but RSM and artificial neural network (ANN) method are compared. Unal et al. studied the abrasive wear behavior of different polymers. For all tested polymers like POM, UHMWPE, PA66 and its composites, the wear rate increased linearly with abrasive distance and grit sizes. Several other studies indicated that Taguchi approach was applied on the abrasive wear behavior of the polymeric
materials including glass/carbon
fibers/fabrics and SiC particles [27-32,35-39,42-45].
There are number of studies on the dry wear behaviour of polymers and its composites [5-21] while there are some works on abrasive
wear for polymers and its composites [22-26; 33-39;42-45], but no study is conducted on the abrasive wear behaviour of PAs using a RSM method, especially for heavy loading conditions. Therefore, the aim of this work is to determine the dry wear behavior of different casting polyamides by a RSM under SiC emery papers and multi-linear regression equation is developed to predict the wear behaviour of polyamides.
Table 1. Chemical, physical and mechanical properties of PAs.
Some properties (Mechanical, physical and
chemical) Material’s types
PA6G PA6E PA6G+ oil
Density (gr/cm3) 1.14 1.14 1.135
Thermal conductivity (W.m-1.K-1) 0.28 0.28 0.28
Rockwell hardness (N.mm2) M85 M88 M82
Compressive strength at % 5 (GPa) 87 110 85
Tensile strength (MPa) 80 93 73
Tensile strain at break (%) 70 50 25
Elastic modulus (MPa) 3300 3550 3000
Water absorption (%) 2.6 2.4 2
Melting points (°C) 220 260 225
Max allowable service
temperature (°C) 160 180 165
2.2 Experimental design
Response surface methodology (RSM) uses a statistical measure of performance to evaluate the optimal parameter settings. In the present work, three parameters such as load (L), speed (S) and tensile stress (T) on the volumetric wear rates (VWR) of the polyamides as control parameters are studied using a Box-Behnken Design (BBD). The BBD requires minimum three levels of each factor for the calculation of the regression coefficients. The total 15 experimental trials are carried out according to the BBD design matrix. In this method, input parameters are controllable and multi-factor analysis is made for optimization of dry wearing control parameters for given responses. The data are combined with the different variables according to the center point of the cube edge at 12 positions and the center of the cube at 3 repetitions. Their codes and levels of control parameters are shown in Table 2.
Table 2. Control factors and their levels (un-coded).
Symbol parametersControl Unit Level 1 Level 2 Level 3
L Applied load N 7 17.5 28
S Sliding speed m/s 0.33 0.66 0.98
T Material tensile
strength MPa 73 80 95
This table indicates that the experimental plan has three levels. Each combination of experiments is repeated three to acquire more accurate results in the process.
2.3 Wear test
Experiments are carried out on polyamides using a pin-on-disc wear testing configuration in accordance with ASTM standard. Counter surface material is an AISI 4140 steel disc by 14 mm in thick, which was heat-treated to give a surface hardness of 59-63 HRC. The counter surface material was ground to a surface finish of approximately 0.40 µm center-line average, but SiC abrasives are attached on the smooth steel disc. The pin is slid in a circular motion against the SiC emery paper on the hardened steel to perpendicular to sliding direction. PA bars are machined into small cylindrical shape with a lathe machine. The pin specimen is ﬁxed to the specimen holder by setting screws. The diameter of the pin is 8 mm with 15 mm in length. Wear tests were carried out at different sliding speeds under three loads of 7, 17.5 and 28 N. The normal load is applied through a spring and lever system. Sliding radius is about 130mm while sliding distances are about 15m, 30m and 45m, respectively. Abrasive paper type was SiC and its grade was 400 grit size. The material loss of samples is calculated from the weight loss method. After the test, the wear pin is cleaned in acetone prior to and after the test, then dried and weighed on a microbalance with 0.1 mg sensitiveness. Each test is performed with a new track of plate. Three replicates are carried out for each material and the results are averaged from the three test runs.
3. RESULTS AND DISCUSSION
3.1 Analysis of wear
was lower for this sample because its increased tensile strength and modulus of elasticity (see Table 2).
Table 3. Experimental plan, run and abrasive dry wear results for the volumetric wear rate.
Main control factors Wear rate
Run L, N S, m/s MPa T,
Volume. wear rate (mm3/m)
Theor. wear rate (mm3/m)
1 7 0.33 83 1.61616 1.8759 13.85
2 28 0.33 83 3.06220 2.9761 2.89
3 7 0.98 83 0.81033 0.8964 9.60
4 28 0.98 83 2.19365 1.9339 13.43
5 7 0.65 73 1.80046 1.4542 23.8
6 28 0.65 73 3.26776 3.2674 0.010
7 7 0.65 93 0.94630 0.9466 0.037
8 28 0.65 93 0.92503 1.2712 27.23
9 17.5 0.33 73 2.74676 2.8332 3.05
10 17.5 0.98 73 2.26557 2.5256 10.29
11 17.5 0.33 93 2.54474 2.2846 11.38
12 17.5 0.98 93 0.65689 0.5704 15.15
13 17.5 0.65 83 1.77210 1.7207 2.98
14 17.5 0.65 83 1.68704 1.7207 1.96
15 17.5 0.65 83 1.70299 1.7207 1.02
Average error (%) 9.112
30 20 10 2.6 2.4 2.2 2.0 1.8 1.6 1.4 1.2 1.0 1.00 0.75
0.50 70 80 90
L M ea n of V ol um et ri c w ea r ra te ( m m 3/ m
) S T
Main Effects Plot for Volumetric wear rate (mm3/m) Fitted Means
Main control factors
Fig. 1. Mean plot for mean volumetric wear rate of PA6G, PA6E and PA6G+oil types of polyamides. Therefore, the formation of heat was prevented by this property between the components that rubbed against each other. The wear became a smaller with the decreasing the elongation. The previous work on the dry wear behaviors of polyamides revealed that optimal factor was obtained for PA6G plus oil type of polyamides against hardened steel . This might be due to testing the lubricated type of sample against the hardened smooth steel and resulting in
formation of transfer layer on the counter face. The sliding velocity and load influenced the frictional heating of polyamide (N6), thereby increasing the wear rate due to increase in the temperature . However, for others polymers like POM, UHMWPE, PA66 and its composites, the wear rate increased linearly with abrasive distance and grit sizes [6,26].
Fig. 2. Interaction plot for mean volumetric wear rate values for the polyamides. Figure 3 shows the surface plot of the volumetric
wear rate vs.interaction parameters under all applied parameters. Figure 3a indicates the VWR vs.L,T while Fig. 3b shows the VWR vs.L,S and Fig. 3c indicates the VWR vs. S,T parameter, respectively. These figures also confirmed the previous Fig. 1, indicating the dominant factor of tensile strength, which is followed by the load.
Fig. 3. Surface plot of volumetric wear rate vs.interaction parameters. (a) VWR vs.L,T; (b) VWR vs.L,S, (c) VWR vs.S,T.
Fig. 5. Residual versus fit values on the volumetric wear rate of the polyamides.
Figure 4 shows the normal plot of standardized effect of process parameters on the average volumetric wear rate of the polyamides. It visually exhibited the degree of effect of each parameter in the obtained results. This figure indicated that the main control factors of A, B, C had a statistically significant effect on the wear of the tested samples. Moreover, Fig. 5 indicates the residual versus fit values on the wear rate of the polyamides. The residual distributed a uniformly around the dot line and its fitted values is lower than 4 while the residual value is about 0.35.
3.2 Analysis of variance (ANOVA)
The ANOVA was used to investigate which design parameters significantly affect the quality characteristic for the wear rate of the polyamides. The results for the sliding wear behavior of polymeric materials under SiC abrasive papers were analyzed and listed in Table 4. This analysis was performed for the 5 % significance level, that is, for the 95 % confidence level. It is clear that factor T had a statistical and physical significance on the wear rate because P-value was lower than 0.05 value, followed by factor L and factor S, respectively.
P-value indicates the degree of influence from each factors. It could be observed that factor T (P-value = 0.003) had a significant effect, followed by factor L (P-value = 0.006) and factor S (P-value = 0.007), respectively. Other factors like square (P=0.514), and two-way interaction factors (P=0.12) did not indicate any significant effects on the dry wear properties. However, the lack of fit value is equal to 0.011, which was lower than 0.05 value. Besides, a contribution of each factor (Pc) on total variations in the last column can be
calculated and shows a degree of influence on the wear results. The contributions of T, L and S were about 33.55, 24.54 and 21.87 %, respectively. However, sliding/abrasive distance was the wear factor that had the highest statistical influence on the dry wear of composites [22,33,35].
3.3 Regression analysis
The correlations between the control parameters like load (L), speed (S), tensile strength of the tested samples (T) and wear rate were found by multiple regressions. The correlations were as follows:
Regression equation in uncoded units,
Volumetric wear rate, VWR (mm3/m) = 1.72 + 0.534 L + 4.29 S - 0.052 T - 0.00054 L*L
+ 2.45 S*S + 0.00074 T*T - 0.0046 L*S (1) - 0.00354 L*T - 0.1082 S*T
Where VWR means is the average volumetric wear rate; Eq. (1) indicated that the wear rate increased with the load and the sliding speed, but it decreased with the increasing material’s tensile strength for testing the composites.
Table 4. Analysis of variance for the wear property of various polyamides.
Source DF Adj.SS Adj.MS F-Value P-value (%) Pc
Model 9 8.797 0.977 8.99 0.013 4.17
Linear 3 7.463 2.487 22.87 0.002 79.8
L 1 2.284 2.284 21.01 0.006 24.5
S 1 2.043 2.043 18.79 0.007 21.8
T 1 3.134 3.134 28.82 0.003 33.5
Square 3 0.284 0.094 0.87 0.514 3.04
L*L 1 0.013 0.013 0.12 0.743 3.04
S*S 1 0.248 0.248 2.28 0.191 2.65
T*T 1 0.019 0.019 0.18 0.686 0.21
Inter. 3 1.049 0.349 3.22 0.120 11.2
L*S 1 0.0009 0.0009 0.01 0.928 0.00
L*T 1 0.553 0.553 5.09 0.074 5.92
S*T 1 0.494 0.494 4.55 0.086 5.29
Error 5 0.543 0.108 5.82
fit 3 0.539 0.179 88 0.011 5.77
error 2 0.0040 0.002
Total 14 9.341 100
Eq. (1) with the substituting the recorded values of the variables. In the predicting of the wear rate, average error was found to be lower than 9.1 %. The use RSM on UHMWPE was successfully developed a model that the filler loading, load and sliding speed had a significant effect on the wear rate and COF of UHMWPE . The second order regression model showed that the load was higher effect than speed and materials type, respectively .
The abrasive/dry sliding wear behavior of three different types of polyamides was investigated in a pin-on-disc tribometer against SiC abrasive clothes using the RSM method under different parameters.
The following conclusions were drawn:
1. The abrasive sliding wear properties of various polyamides samples were determined using a Box-Behnken Design (BBD) of response surface methodology. The volumetric wear rate decreased with increasing the tensile strength and speed, but it increased with the load.
2. Among the tested samples, PA6E samples showed the higher wear resistance than that of others at all conditions because of higher tensile strength and modulus of elasticity. 3. ANOVA exhibited that the tensile strength
was the most effective factor on the wear rate of PAs (P=33.55%), followed by the factor L (P=24.45%) and the factor S (P=21.87%), respectively.
 S.S. Prabu, S. Prathiba, A. Sharma, S. Garg, G. Manikandan, C. Sriram, Investigation on Adhesive Wear Behavior of Industrial Crystalline And
Semi-Crystalline Polymers Against Steel Counter Face,
International Journal of ChemTech Research, vol. 6, no. 7, pp. 3422-3430, 2014.
 A. Kaştan, H. Unal, Abrasive Wear Behavior of Polyamide6/Polyproylene/Nanoclay Composites,
Romanian Journal of Materials, vol. 47, no. 2, pp. 237-243, 2017.
 M.J. Neale, M. Gee, Guide To Wear Problems and
Testing For Industry, New York, USA: William
Andrew Publishing, 2001.
 T. Mang, W. Dresel, Lubricants And Lubrication, Willey-VCH, 2007.
 Z.B. Chen, T.S. Li, Y.L. Yang, Y. Zhang, S.Q. Lai, The Effect of Phase Structure on The Tribological
Properties of PA66/HDPE Blends, Macromolecular
Materials and Engineering, vol. 289, iss. 7, pp. 662– 671, 2004, doi: 10.1002/mame.200300266  Z. Chen, T. Li, Y. Yang, X. Liu, R. Lv, Mechanical
And Tribological Properties of PA/PPS Blends,
Wear, vol. 257, iss. 7-8, pp. 696–707, 2004, doi: 10.1016/j.wear.2004.03.013
 J. Liu, H. Lin, H.L. Yi, T. Wei, B.C. Zheng, The Influence of Modified Polytetrafluoroethylene(PTFE)
on The Properties of PA6/PTFE Blends, Applied
Mechanics and Materials, vol. 662, pp. 38-45, 2014,
doi: 10.4028/www.scientific.net/AMM.662.38  M. Brožek, Selected Plastics Wear Resistance to
Bonded Abrasive Particles Compared to Some
Ferrous Materials, ACTA universitatis
agriculturae et silviculturae mendelianae brunensis, vol. 63, pp. 387-393, 2015, doi: 10.11118/actaun201563020387
 Y. Şahin, S. Yalçınkaya, H. Mirzayev, The effect of load on the tribological property of polyacetal
and metallographic observation, in Proceedings
of the International Symposium of Mechanism and Machine Science, 11-14 September 2017, AzCIFToMM, Technical University, Baku, Azerbaijan, pp. 167-174.
 A. Abdelbary, M.N. Abouelwafa, I. El Fahham, AI. Gomaa, A New Reciprocating Tribometer for Wear Testing under Different ﬂuctuating Loading
Conditions, Alexandria Engineering Journal, vol.
43, no. 5, pp. 615–619, 2004.
 A.G.A. Rosa, J.A. Moreto, M.D. Manfrinato, L.S. Rossino, Study on Friction and Wear Behavior of SAE 1045 Steel, Reinforced Nylon 6.6 And NBR
Rubber Used in Clutch Disks, Materials Research,
vol. 17, no. 6, pp. 1397-1403, 2014, doi: 10.1590/1516-1439.282714
 Z. Zalisz, P.H. Vroegop, R. Bosma, A Running-in Model for the Reciprocating Sliding of Nylon 6.6
Against Stainless Steel, Wear, vol. 121, iss. 1, pp. 71–
93, 1988, doi: 10.1016/0043-1648(88)90032-4  Y.Q. Wang, J. Li, Sliding Wear Behavior And
Mechanism of Ultrahigh Molecular Weight
Polyethylene, Materials Science and Engineering:
A, vol. 266, iss. 1-2, pp. 155–160, 1999, doi: 10.1016/S0921-5093(99)00040-4
 B.-B. Jia, T.-S. Li, X.-J. Liu, P.-H. Cong, Tribological Behaviors of Several Polymer–Polymer Sliding Combinations under Dry Friction and Oil-Lubricated
Conditions, Wear, vol. 262, iss. 11-12, pp. 1353–
 H. Unal, A. Mimaroglu, Influence of Test Conditions
on the Tribological Properties of Polymer, Industrial
Lubrication and Tribology, vol. 55, no. 4, pp. 178– 183, 2003, doi: 10.1108/00368790310480362  G. Kalácska, An Engineering Approach to Dry
Friction Behaviour of Numerous Engineering
Plastics with Respect to the Mechanical Properties,
eXPRESS Polymer Letters, vol. 7, no. 2, pp. 199-204, 2013, doi: 10.3144/expresspolymlett.2013.18  A.L. Gasparina, L.L. Corsoa, E.K. Tentardini, R.C.R. Nunesc, M.M.C. Forted, R.V.B. Oliveira, Polyamide
Worm Gear: Manufacturing and Performance,
Materials Research, vol. 15, no. 3, pp. 483-489, 2012, doi: 10.1590/S1516-14392012005000056  S. Yu, H, Hu, J. Yin, Effect of Rubber on Tribological
Behaviors of Polyamide 66 under Dry and Water
Lubricated Sliding, Wear, vol. 265, iss. 3-4, pp. 361–
366, 2008, doi: 10.1016/j.wear.2007.11.006  S.E. Franklin, Wear Experiments with Selected
Engineering Polymers and Polymer Composites
under Dry Reciprocating Sliding Conditions,
Wear, vol. 251, iss. 1-12, pp. 1591–1598, 2001,
 Y. Şahin, Wear Analysis of Polyamides Based on a
Statistical Approach, International Journal of
Materials and Product Technology (IJMPT), vol. 54, iss. 1-3, pp. 107-125, 2017, doi: 10.1504/IJMPT.2017.080561
 Y. Şahin, D.B. Patrick, Dry sliding wear behavior
of polyamides by taguchi method, 2016, in The
6th International Conference on Advance Materials & Research (ICAMR 2016), January 22-24, Torino, Italy, vol. 689, pp. 81-85.
 V. Pejakovic, R. Jisa, F. Frank, Abrasion Resistance of Selected Commercially Available Polymer
Materials, Tribologia-Finnish Journal of
Tribology, vol. 33, no. 1, pp. 21-27, 2015.
 P.H. Shipway, N.K. Ngao, Microscale Abrasive
Wear of Polymeric Materials, Wear, vol. 255, iss.
1-6, pp. 742-750, 2003, doi: 10.1016/S0043-1648(03)00106-6
 F. Kahraman, U. Esme, M.K. Kulekci, S. Ocalir,
Abrasive Wear and Frictional Behavior of
Polyoxymethylen, Wear testing, vol. 59, iss. 10,
pp. 880-883, 2017, doi: 10.3139/120.111083  A. Sağbas, F. Kahraman, U. Esme, Modellig And
Predicting Abrasive Behavior of Polymethylenes
using RSM and ANN Method, Metalurgija, vol. 48,
no. 2, pp. 117-120, 2009.
 H. Unal, U. Sen, A. Mimaroglu, Abrasive Wear
Behaviour of Polymeric Materials, Materials &
Design, vol. 26, iss. 8, pp. 705–710, 2005, doi: 10.1016/j.matdes.2004.09.004
 S. Basavarajappa, K.V. Arun, J.P. Davim, Effect of Filler on Dry Wear Behavior of Polymer Matrix
Composites, J. Macromolecular Materials&
Engineering, vol. 8, no. 5, pp. 379-391, 2009, doi: 10.4236/jmmce.2009.85034
 G. Srinath, R.Gnanamoorthy, Sliding Wear Performance of Polyamide 6 Clay Nanocomposites
in Water, Composite Science Technology, vol. 67,
iss. 3-4, pp. 399–405, 2007, doi: 10.1016/j.compscitech.2006.09.004
 J.H. Byett, C. Allen, Dry Sliding Wear Behaviour of
Polyamide 66 And Polycarbonate Composites,
Tribology International, vol. 25, iss. 4, pp. 237– 246, 1992, doi: 10.1016/0301-679X(92)90061-Q  L. Chang, Z. Zhang, H. Zhang, A.K. Schlarb, On the Sliding Wear of Nanoparticle ﬁlled Polyamide 66
Composites, Composite Science and Technology,
vol. 66, iss. 16, pp. 3188–3198, 2006, doi: 10.1016/j.compscitech.2005.02.021
 J. Wang, G. Mingyuan, Wear Properties and Mechanisms of Nylon and
Carbon-ﬁber-Reinforced Nylon in Dry and Wet Conditions,
Journal of Applied Polymer Science, vol. 93, iss. 2, pp. 789–95, 2004, doi: 10.1002/app.20483  J. Khedkar, I. Negulescu, E.I. Meletis, Sliding Wear
Behaviour of PTFE Composites, Wear, vol. 252,
iss. 5-6, pp. 361–369, 2002, doi: 10.1016/S0043-1648(01)00859-6
 J. Rajesh, J. Bijwe, U.S. Tewari, Abrasive Wear
Performance of Various Polyamides, Wear, vol.
252, iss. 9-10, pp. 769-776, 2002, doi: 10.1016/S0043-1648(02)00039-X
 J. Sukumaran, R. Keresztes, G. Kalácska, H. Almaliki, P.D. Neis, P. De Baets, Extruded And Injection Moulded Virgin PA 6/6 as Abrasion
Resistant Material, Advances in Tribology, vol.
2017, p. 9, 2017, doi: 10.1155/2017/1035017
 C. Anand, S.P. Kumaresha, Influence of Titanium Carbide on the Three-Body Abrasive Wear Behaviour of Glass-Fabric Reinforced Epoxy
Composites, Advanced in Materials, vol. 1, iss. 1,
pp. 9-15, 2012, doi: 10.11648/j.am.20120101.12
 N. Chand, U.K. Dwivedi, High Stress Abrasives Wear
Study on Bamboo, Journal of Materials Processing
Technology, vol. 183, iss. 2-3, pp. 155–159, 2007,
 K.S. Rao, Modelling and Analysis of Abrasive Wear Performance of Glass Epoxy Composites using
Taguchi Approach, International Journal of
Metallurgy & Materials Science Engineering (IJMMSE), vol. 3, iss. 5, pp. 19-28, 2013.
 B.R. Raju, R.P. Swamy, B. Suresha,K.N. Bharath,
Composites, Advances in Polymer Science and Technology: An International Journal, vol. 2, no. 4, pp. 51-57, 2012.
 B. Suresha, K.N.S. Kumar, Investigations on Mechanical and Two-Body Abrasive Wear Behavior of Glass/Carbon Fabric Reinforced Vinyl Ester
Composites, Materials & Design, vol. 30, iss. 6, pp.
2056–2060, 2009, doi:
 B.P. Chang, H. Md Akil, R. Bt Nasir, A. Khan,
Optimization on Wear Performance of UHMWPE Composites Using Response Surface Methodology,
Tribology International, vol. 88, pp. 252-262, 2015, doi: 10.1016/j.triboint.2015.03.028  C.Z. Liu, L.Q. Ren, J. Tong, T.J. Joyce, S.M. Green,
R.D. Arnell, Statistical Wear Analysis of
PA-6/UHMWPE Alloy, UHMWPE and PA-6, Wear, vol.
249, iss. 1-2, pp. 31–36, 2001, doi: 10.1016/S0043-1648(00)00555-X
 Y. Şahin, Analysis of Abrasive Wear Behavior of
PTFE Composite Using Taguchi’s Technique,
Cogent Engineering, vol. 2, iss. 1, pp. 1-15, 2015,
 S. Basawarajappa, A.G.K. Joshi, V. Arun, A.P. Kumar, P.M. Kumar, Three-Body Abrasive Wear Behavior of Polymer Matrix Composites Filled
With SiC Particles, Polymer-Plastics Technology
Engineering, vol. 49, iss. 1, pp. 8–12, 2009, doi: 10.1080/03602550903206407
 R.B.N. Kumar, B. Suresha, M. Venkataramareddy,
Effects of Particulate Fillers on Mechanical And
Abrasive Wear Behavior of Polyamide
66/Polypropylene Nanocomposites, Materials &
Design, vol. 30, iss. 9, pp. 3852–3858, 2009, doi: 10.1016/j.matdes.2009.01.034
 Y.Şahin, E. Erdil, H.Şahin, The tribological wear behavior of carbon fabric-reinforced epoxy
composites. In: Editors (Alizade Rasim , Gokhan
Kiper),Proceedings of the International Symposium of Mechanism and Machine Science, Azerbaijan Technical University, 11-14 September 2017, AzCIFToMM, Baku, Azerbaijan, pp. 174-181.
 Polyamids, available at: